Imperial College London
Department of Chemical Engineering and Chemical Technology
Thin Film Composite Membranes by Interfacial
Polymerization for Organic Solvent Nanofiltration
María Fernanda Jiménez Sólomon
Supervisor: Prof. Andrew G. Livingston
A thesis submitted for the degree of Doctor of Philosophy of Imperial College
London and the Diploma of Imperial College London
I certify that the work in this thesis is my own and that the work of others is
“The copyright of this thesis rests with the author and is made available
under a Creative Commons Attribution Non-Commercial No Derivatives
licence. Researches are free to copy, distribute or transmit the thesis on the
condition that they attribute it, that they do not use it for commercial purposes
and that they do not alter, transform or build upon it. For any reuse or
redistribution, researches must make clear to others the licence terms of this
To Ricardo, Lorena, Rodrigo, Jorge, Ana, Memé y el Güero
One of the challenges of current organic solvent nanofiltration (OSN) membranes is to improve permeability in polar and non-polar solvents without compromising selectivity. Here, the development of a new generation of OSN membranes: High flux Thin Film Composite membranes (TFC) via interfacial polymerization (IP), is proposed. This thesis offers a comprehensive study that analyses the relationship of OSN high flux TFC membrane formation and post-formation parameters, morphology, structure and surface polarity, to membrane functional performance in both polar and non polar solvents. The dissertation starts with the development of novel high flux TFC membranes for polar aprotic solvents to address the trade-off between permeability and selectivity. This is accomplished by using two different approaches: (a) incorporation of polyethylene glycol inside the pores of the support prior to the IP reaction, and; (b) post-treatment of the TFC membranes with an “activating solvent”. Subsequently, a detailed analysis of membrane performance and morphology, considering the aforementioned approaches was conducted, resulting in dramatically increased solvent fluxes without compromising rejection. Additionally, a detailed study to manipulate molecular weight cut-off (MWCO) of these TFC membranes was carried out and successfully achieved by using different amines in the IP reaction. Next, novel high flux hydrophobic TFC membranes via IP with tuned MWCO for non-polar solvents were developed, elucidated and studied. The surface properties of hydrophilic TFC OSN membranes were modified by capping the free acyl chloride groups on their surface with different monomers containing hydrophobic groups. A detailed study on surface polarity and membrane performance was undertaken, suggesting that surface chemistry plays an important role in solvent permeation. The membrane performance was compared to commercial OSN integrally skinned asymmetric (ISA) and TFC rubber-coated membranes. In the next stage of this thesis, the effects of different support membranes on TFC membrane formation and functional performance were studied for both polar and non-polar solvents. It was found that support membranes have an effect on TFC membrane formation and solvent permeation. Finally, to increase permeability even further without a requirement for treating the TFC membrane with an activating solvent, highly porous TFC membranes have been developed via IP by controlling the structure of the top layer at a molecular level. This was achieved by incorporating a monomer with a contorted structure during the IP reaction, resulting in a highly porous polymer network. It is believed high flux TFC OSN membranes prepared by interfacial polymerization may offer new degrees of freedom in membrane design, which could lead to the next generation of high performance OSN membranes.
I would like to thank my supervisor Professor Andrew G. Livingston for his encouragement and support throughout the course of my PhD. It has been a privilege working and learning from you. I am also grateful to all my colleagues in the Livingston’s group who were always there to advise me and support me. Special thanks to Dr. Yogesh for working closely with me during many stages of my PhD, to Marta for working with me during the research on TFC-PIMs membranes, and to Iwona, Humera and Asia for their important input in my work, and their support during my PhD.
I would like to thank those who technically contributed to this work, Jeong for conducting GPC analyses, and Joanna and Elin for collaborating with me.
I would like to acknowledge financial support provided by the 7Th Framework Programme of the European Commission’s Marie Curie Initiative (NEMOPUR project, grant No. 214226-2).
Special thanks to my friends Elisa, Armando, David, Iwona, Fabian, Alonso, Ana and Ioscani, who were always there to support me. I am also grateful to all my Friends from Mexico, who despite the distance have always been there for me: Roberto, Jesica, Mariana, Alexandra, Tanya, Maricarmen, Alejandro, Adri, and Andrea.
To the above-mentioned and many other unnamed colleagues and friends, who have also contributed to the completion of this work and gave me their support, I extend my sincere thanks.
Thanks Tom (: for your support and all the good times we had during my write-up period.
Finalmente quiero agradecerle a mi familia, a quien extraño todos los días. Gracias a su amor, su gran apoyo y su amistad tengo la oportunidad de celebrar este éxito, el cual también es suyo.
Parts of this thesis have been published or submitted for publication:
M.F. Jimenez Solomon, Y. Bhole, and A.G. Livingston, High flux membranes for organic solvent nanofiltration (OSN)—Interfacial polymerization with solvent activation. J. Membr. Sci. 423–424 (2012) 371-382.
M.F. Jimenez Solomon, Y. Bhole, and A.G. Livingston, High flux hydrophobic membranes for organic solvent nanofiltration (OSN)—Interfacial polymerization, surface modification and solvent activation. J. Membr. Sci. 434 (2013) 193-203.
Joanna Stawikowska, M.F. Jimenez Solomon, Y. Bhole, and A.G. Livingston, Nanoprobe contrast agents to elucidate the structure of thin film composite nanofiltration membranes. J. Membr. Sci. 442 (2013) 107-118.
György Székely, Patrizia Marchetti, M.F. Jimenez Solomon, and A.G. Livingston, Nanofiltration Membranes in Organic Solvents. Encyclopedia of Membrane Science and Technology, Wiley (2013) Accepted.
M.F. Jimenez Solomon, Patricia Gorgojo, and A.G. Livingston, Beneath the surface: Influence of supports on thin film composite membranes by interfacial polymerization for organic solvent nanofiltration. J. Membr. Sci. (2013) in Press.
Parts of this thesis have resulted in patent applications:
M.F. Jimenez Solomon, Y. Bhole, and A.G. Livingston, UK Patent application No 1117950.4, Membranes for separation (2010).
M.F. Jimenez Solomon, Y. Bhole, and A.G. Livingston, UK Patent applicationNo 1012083.0, Thin Film Composite Membranes for separation (2011).
List of Figures
Figure 1. Schematic representation of polymeric membranes; (a) integrally skinned
asymmetric membrane; (b) thin film composite membrane. ... 5
Figure 2. RO membranes performance. ... 5
Figure 3. Membrane casting. ... 8
Figure 4. Schematic representation of TFC membrane formation. ... 10
Figure 5. Chemical structure of polyamide FT-30 membrane. ... 11
Figure 6. Diagram of typical TFC membrane production process. ... 19
Figure 7. Chemical potential (µi), pressure (p), and solvent activity (γici) profiles for pressure-driven permeation through a membrane according to (a) solution-diffusion and (b) pore-flow transport models. ... 38
Figure 8. SEM images of surface of TFC membranes. (a) PESf- TFC-MPD membrane; (b) TFC-MPD membrane prepared on crosslinked polyimide support; (c) TFC-PIP membrane prepared on crosslinked polyimide support. ... 53
Figure 9. ATR-FTIR spectra of crosslinked PI support and TFC-MPD membrane. ... 54 Figure 10. ATR-FTIR spectra of crosslinked P84 UF supports with and without PEG. ... 56
Figure 11. MWCO curves and fluxes of TFC membranes prepared on a crosslinked polyimide support membrane with and without PEG as conditioning agent, and with and without post- treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in methanol has been performed at 30 bar and 30°C. (a) No PEG, no activating solvent treatment; (b) No PEG, with activating solvent treatment; (c) With PEG, no activating solvent treatment; (d) With PEG, with activating solvent treatment. ... 57
Figure 12. MWCO curve and flux of TFC membranes prepared on a crosslinked polyimide support membrane without (a) and with (b) PEG as conditioning agent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in DMF has been performed at 30 bar and 30°C. ... 58
Figure 13. Repeatability of MWCO curve and flux of TFC membranes prepared on a crosslinked polyimide support membrane with PEG as conditioning agent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in DMF has been performed at 30 bar and 30°C. ... 59
Figure 14. SEM images of TFC OSN membranes. (a) Shows the cross-section of TFC-MPD before DMF treatment; (b) Shows the cross-section of TFC-TFC-MPD after treating with DMF; (c) Shows the surface of TFC-MPD membrane before treating with DMF; (d) is the surface of TFC-MPD after treating with DMF. ...
Figure 15. MWCO curve and flux of TFC-MPD membranes without (a) and with (b) treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising
polystyrene oligomers dissolved in acetone performed at 30 bar and 30°C. ... 62
Figure 16. MWCO curves and fluxes of TFC-MPD membranes after treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in ethyl acetate or toluene has been performed at 30 bar and 30°C. (a) ethyl
acetate as solvent; (b) toluene as solvent. ... 63
Figure 17. MWCO curves and fluxes of membranes after treatment with DMF as an activating solvent. Comparative study between TFC-MPD membranes and commercial integrally skinned asymmetric OSN membranes (DM150). Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in THF or acetone has been performed at 30
bar and 30°C. (a) THF as solvent; (b) acetone as solvent. ... 63
Figure 18. MWCO curves and flux of TFC membranes prepared with different amines after immersion in DMF as an activating solvent. Nanofiltration of a feed solution
comprising alkanes dissolved in THF performed at 30 bar and 30°C. ... 65
Figure 19. MWCO curves and flux of TFC membranes prepared with different amines after immersion in DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in acetone performed at 30 bar and 30°C. (a)
amine is MPD; (b) amine is PIP; (c) amine is HDA. ... 65
Figure S1. Electromicrographs of PA/XP84 TFC membrane (courtesy of J. Stawikowska). (a) TEM cross sectional image of the PA/P84 membrane after filtration from the surface
side, (b) and the open side... 67
Figure S2. High magnification TEM cross-sectional images of the PA composite separation layer. Three images acquired from different regions (courtesy of J.
Stawikowska). ... 68
Figure 20. Strategies for Hydrophobic TFC membrane formation. ... 77
Figure 21. MWCO curves and fluxes of TFC membranes after treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in toluene has been performed at 30 bar and 30°C. (a) Comparison study between control TFC membrane and commercial integrally skinned asymmetric OSN membrane (SM 122); (b) TFC membrane capped with fluoro-alkylamine; (c) TFC membrane capped with silicone-alkylamine; (d) TFC membrane capped with
fluoro-alkylacylchloride. ………... 81
Figure 22. MWCO curves and fluxes of TFC membranes after treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in THF performed at 30 bar and 30°C. (a) Control TFC membrane; (b) TFC membrane capped with fluoro-alkylamine; (c) TFC membrane capped with
Figure 23. MWCO curves and fluxes of TFC membranes after treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in Toluene has been performed at 30 bar and 30°C. (a) Control TFC membrane prepared by 3 steps IP; (b) 3-steps IP TFC membrane capped with alkylacylchloride; (c) Control TFC membrane; (d) TFC membrane capped with
fluoro-alkylacylchloride. ………..……….. 84
Figure 24. MWCO curves and fluxes of TFC membranes after treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers
dissolved in Ethyl acetate performed at 30 bar and 30°C. ………..……… 86
Figure 25.MWCO curves and fluxes of TFC membranes after treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in Toluene performed at 30 bar and 30°C. Comparison study between TFC
membranes and commercial rubber coated TFC OSN membranes (S380). ... 87
Figure 26. MWCO curves of crosslinked polyimide (XP84(DMSO)) and poly(ether ether
ketone) (PEEK) UF support membranes. Filtration of feed solutions comprising dextran
dissolved in water has been performed at 2 bar and 25°C. ... 100
Figure 27. Flux curves of crosslinked polyimide (XP84(DMSO)) and poly(ether ether ketone)
(PEEK) UF support membranes. Filtration of feed solutions comprising dextran dissolved
in water has been performed at 2 bar and 25°C. ... 100
Figure 28. AFM topographical images of UF support membranes revealing changes in surface roughness: (a)XP84(DMSO) membrane without PEG , (b) XP84(DMSO) membrane with
PEG, (c) PEEK membrane without PEG, (d) PEEK membrane with PEG. ……… 101
Figure 29. The data shown here has been reproduced from Figure 11 for convenience of comparison. MWCO curves and fluxes of TFC membranes prepared on a crosslinked polyimide support membrane with and without PEG as conditioning agent, and with and without post-treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in methanol has been performed at 30 bar and 30°C. (a) No PEG, no activating solvent treatment; (b) No PEG, with activating solvent treatment; (c) With PEG, no activating solvent treatment; (d) With PEG, with activating
solvent treatment. ... 105
Figure 30. SEM images of TFC membranes revealing changes in surface morphology: (a) TFC membrane prepared on XP84(DMSO) without PEG, (b) TFC membrane prepared on XP84(DMSO) with PEG, (c) TFC membrane prepared on PEEK without PEG, (d) TFC
membrane prepared on PEEK with PEG. ………. 106
Figure 31. SEM images of TFC membranes revealing changes in surface morphology: (a) TFC membrane prepared on XP84(DMSO) without PEG post-treated with DMF, (b) TFC membrane prepared on XP84(DMSO) with PEG post-treated with DMF, (c) TFC membrane prepared on PEEK without PEG post-treated with DMF, (d) TFC membrane prepared on PEEK with PEG post-treated with DMF. Post-treatment was done by immersion in DMF for
Figure 32. MWCO curves and fluxes of TFC membranes prepared on a poly (ether ether ketone) (PEEK) support membrane with and without PEG as conditioning agent, and with and without post-treatment with DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in methanol has been performed at 30 bar and 30°C. (a) No PEG, no activating solvent treatment; (b) No PEG, with activating solvent treatment; (c) With PEG, no activating solvent treatment; (d) With PEG, with
activating solvent treatment. ... 108
Figure 33. Comparison MWCO curves and fluxes of commercial membrane Duramem® 150 and TFC membranes prepared on either a poly (ether ether ketone) (PEEK) or a crosslinked polyimide support membrane impregnated with PEG as conditioning agent, and with post-treatment using DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in THF has been performed at 30 bar
and 30°C. ... 109
Figure 34. Comparison MWCO curves and fluxes of commercial membrane Starmem™
122 and hydrophobic TFC membranes prepared on either a poly (ether ether ketone) (PEEK) or a crosslinked polyimide support membrane impregnated with PEG as conditioning agent, and with post-treatment using DMF as an activating solvent. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in toluene has
been performed at 30 bar and 30°C. ... 110
Figure 35. MWCO curves and flux of TFC-PIMs membranes prepared on a crosslinked polyimide (PI) support membrane with PEG as conditioning agent, and with and without post-treatment in the oven at 85°C for 10 minutes and commercial membrane DM300. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in acetone
has been performed at 30 bar and 30°C. ... 119
Figure 36. MWCO curves and flux of TFC-PIMs membranes prepared on a crosslinked polyimide (PI) support membrane with PEG as conditioning agent, and with and without post-treatment in the oven at 85°C for 10 minutes. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in methanol has been performed at 30 bar
and 30°C. ... 120
Figure 37. MWCO curves and flux of TFC-PIMs membranes prepared on a crosslinked polyimide (PI) support membrane with PEG as conditioning agent, and with and without post-treatment in the oven at 85°C for 10 minutes. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in DMF has been performed at 30 bar and 30°C. ... 121
Figure 38. MWCO curves and flux of TFC-PIMs membranes prepared on a crosslinked polyimide (PI) support membrane with PEG as conditioning agent, and with and without post-treatment in the oven at 85°C for 10 minutes and commercial membranes DM500 and DM900. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved
in THF has been performed at 30 bar and 30°C. ... 121
Figure 39. MWCO curves and flux of TFC-PIMs membranes prepared on a crosslinked polyimide (PI) support membrane with PEG as conditioning agent, and with and without post-treatment in the oven at 85°C for 10 minutes. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in toluene has been performed at 30 bar and
Figure 40. MWCO curves and flux of TFC-PIMs membranes prepared on a poly(ether ether ketone) (PEEK) support membrane with PEG as conditioning agent, and with post-treatment in the oven at 85°C for 10 minutes. Nanofiltration of a feed solution comprising polystyrene oligomers dissolved in acetone, THF or toluene performed at 30 bar and 30°C;
(a) acetone as a solvent; (b) THF as a solvent; (c) toluene as a solvent. ... 124
Figure 41. Permeate flux of TFC OSN membranes at 30bar and 30°C over 1 week
operation. ... 130
Figure 42. Permeate flux of DM200 membranes at 30bar and 30°C over 1 week
operation. ... 130
Figure 43. Diafiltration modelling of TFC-OSN membranes based on initial rejection data... 132
Figure 44. Diafiltration modelling of DM200 membranes based on initial rejection data….... 133
Figure 45. Gas separation performance of TFC-PIMs membrane prepared on a PEEK support membrane. (a) shows CO2/N2 selectivity vs. CO2 permeability; (b) shows CO2/CH4
List of Tables
Table 1. Polymers used to prepare solvent stable UF support membranes. ... 23
Table 2. Summary on membrane characterization. ... 36
Table 3. Membrane codes for the TFC membranes. ... 47
Table 4. Contact angle of supports with and without PEG. ... 56
Table 5. TFC-MPD membranes flux after post-treatment in different solvents. ... 66
Table 6. Solutions used for the preparation of TFC membranes. ... 74
Table 7. Membrane codes. ... 74
Table 8. Contact angle of TFC membranes. ... 79
Table 9. Surface Elemental Composition. ... 79
Table 10. Membrane codes. ... 94
Table 11. Repeatability analysis. ... 97
Table 12. PEG uptake. ... 99
Table 13. Mercury porosimetry a and N2 adsorption b results. ... 99
Table 14. Contact angle of UF supports with and without PEG. ... 99
Table 15. A quantitative summary of surface roughness. ………... 101
Table 16. Membrane codes for TFC-PIMs and commercial membranes. ... 117
Table 17. Membranes identification codes. ... 128
Table 18. Rejection of Molecule A at 30bar and ~30°C over 1 week operation. ... 131
Table 19. Rejection of Molecule B at 30bar and ~30°C over 1 week operation. ... 131
List of acronyms and abbreviations
AFM Atomic force microscopy
APIs Active Pharmaceutical Ingredients
ATR-IR Attenuated total reflection IR spectroscopy BA 3,5-diaminobenzoic acid
CNTs Carbon nanotubes CSA Camphor sulfonic acid
DCM Dichloromethane DMAc Dimethylacetamide DMDA dimethylenediamine DMF N,N-dimethylformamide DMSO Dimethylsulfoxide EA Ethyl acetate
FT-IR Fourier transfer IR spectroscopy
HDA 1,6-hexamethylenediamine IP Interfacial polymerization IPC Isophthaloyl chloride
ISA Integrally skinned asymmetric
JS Joanna Stawikowska
LLE Liquid-liquid extraction MBRs Membrane bioreactors MEK Methyl ethyl ketone
MET Membrane Extraction Technology MFJS Maria F. Jimenez Solomon
MIBK Methyl isobutyl ketone
MSA Methane sulfonic acid MWCO Molecular weight cut-off
NMDA 1,9-nonamethylenediamine NMP N-methyl pyrrolidone
OSN Organic Solvent Nanofiltration
PAA Polyacrylic acid
PAH Poly(amide hydrazide) PAI Poly(amide imide)
PALS Positron annihilation lifetime spectroscopy PAN Polyacrylonitrile
PAS Positron annihilation spectroscopy
PDMS Polydimethylsiloxane PEA Poly(ether amide) PEBAX Poly(ether-b-amide) PEEK Poly(ether ether ketone) PEG Polyethylene glycol
PEI Polyethyleneimine PESf Polyethersulfone
PIMs Polymers with intrinsic microporosity
PPESK Poly(phthalazinone ether sulfone ketone) PPO Poly(2,6-dimethyl-1,4-phenyleneoxide)
PS Styrene oligomers
PUA Poly(urea amide)
PVA Poly(vinyl alcohol) PVDF Poly(vinylidene fluoride)
RMS Root mean-square
RO Reverse Osmosis
SEM Scanning electron microscopy SLS Sodium lauryl sulfate
S-MPD m-phenylenediamine-5-sulfonic acid
SPPESK Sulfonated poly(phthalozinone ether sulfone ketone)
TEM Transmission electron microscopy TFC Thin film composite
THF Tetrahydrofuran TMC Trimesoyl chloride TPC Terephthaloyl chloride TPC Terephthaloyl chloride TTS 5,5’,6,6’-tetrahydroxy-3,3,3’,3’-tetramethyl-1,1’-spirobisindane UF Ultrafiltration
Chapter 1. Research motivation and thesis structure. ...1
Chapter 2. Literature review. ...4
2.1 Background. ... 4
2.1.1 Membrane development for reverse osmosis. ... 5
2.1.2. Influence of external parameters on membrane performance. ... 6
2.2 Polymeric membranes. ... 7
2.2.1 Integrally skinned asymmetric membranes. ... 7
2.2.2 Thin Film Composite membranes. ... 8
2.2.3 Post-treatment of polymeric membranes. ... 8
2.2.4 Advantages over ISA nanofiltration membranes. ... 9
2.3 TFC membranes prepared by interfacial polymerization. ... 10
2.3.1 Theoretical model of interfacial polymerization. ... 11
2.3.2 Monomers used during IP to prepare TFC membranes. ... 12
2.3.3 Effects of additives, complexing agents and aprotic solvents during the IP reaction on TFC membrane performance. ... 16
2.3.4 Post-treatment of TFC-IP membranes. ... 18
2.4 TFC membranes prepared by dip-coating. ... 19
2.5 Organic Solvent Nanofiltration. ... 20
2.5.1 OSN membranes. ... 20
2.5.2 Research work on polymeric ISA membranes for OSN. ... 21
2.5.3 Research work on TFC membranes for OSN. ... 22
2.5.4 Novel NF membranes with OSN potential. ... 26
2.5.5 Commercial OSN polymeric membranes. ... 27
2.6 Membrane characterization. ... 29
2.6.1 Functional performance. ... 30
2.6.2 Physical-chemical characterization. ... 30
Chapter 3. Project objectives. ...39
Objective 1. Development of high flux TFC OSN membranes for applications in polar solvents via IP. ... 39
Objective 2. Development of high flux TFC OSN membranes for applications in non- polar solvents via IP. ... 40
Objective 3. Study the influence of support membranes on formation and performance of novel TFC OSN membranes by IP. ... 41
Objective 4. Develop new high free volume TFC OSN membranes via IP. ... 41
Objective 5. High flux TFC OSN membranes for the purification of Active Pharmaceutical Ingredients. ... 42
Chapter 4. High Flux Membranes for Organic Solvent Nanofiltration-
Interfacial Polymerization with Solvent Activation. ...43
4.1 Introduction. ... 43
4.2 Experimental. ... 45
4.2.1 Materials. ... 45
4.2.2 Preparation of crosslinked PI UF support membranes. ... 46
4.2.3 Preparation of polyamide thin film composite membranes. ... 47
4.2.4 Treatment of TFC membranes with activating solvent. ... 48
4.2.5 Membrane Characterization. ... 48
4.2.6 Membrane performance. ... 50
4.3 Results and discussion. ... 51
4.3.1 Characterization of TFC OSN membranes. ... 51
4.3.2 Effects of impregnating UF supports with PEG. ... 55
4.3.3 Treatment with activating solvent. ... 57
4.3.4 Controlling permeation pathway dimensions of TFC OSN membranes. ... 64
4.3.5 DMSO as an alternative to DMF as activating solvent. ... 66
4.4 Conclusion. ... 66
4.5 Supplementary information. ... 67
Chapter 5. High Flux Membranes for Organic Solvent Nanofiltration-
Interfacial Polymerization, Surface modification and Solvent
5.1 Introduction. ... 70
5.2 Experimental. ... 72
5.2.1 Materials. ... 72
5.2.2 Preparation of crosslinked PI UF support membranes. ... 73
5.2.3 Preparation of polyamide thin film composite membranes. ... 73
5.2.5 Membrane Characterization. ... 78
5.2.6 Membrane performance. ... 78
5.3 Results and discussion. ... 79
5.3.1 TFC OSN membranes characterization. ... 79
5.3.2 Membrane performance. ... 80
5.4 Conclusion. ... 87
Chapter 6. Beneath the surface: Influence of supports on thin film
Composite membranes by interfacial polymerization for
Organic Solvent Nanofiltration. ...89
6.1 Introduction. ... 90
6.2 Experimental. ... 92
6.2.1 Materials. ... 92
6.2.2 Preparation of crosslinked PI UF support membranes. ... 93
6.2.3 Preparation of PEEK UF support membranes. ... 93
6.2.4 Preparation of polyamide thin film composite membranes. ... 93
6.2.5 Treatment of TFC membranes with activating solvent. ... 94
6.2.6 Membrane Characterization. .... 95
6.2.7 UF support membranes performance. ... 96
6.2.8 Membrane performance. ... 97
6.3 Results and discussion. ... 98
UF support membranes. ... 98
6.3.1 PEG uptake, mercury porosimetry and BET analyses. ... 98
6.3.2 UF membrane performance. ... 99
6.3.3 AFM-surface roughness analysis. ... 101
TFC membranes. ... 102
6.3.4 Contact angle. ... 102
6.3.5 TFC membranes performance and characterization. ... 102
6.3.6 Impacts of support on permeability for hydrophilic and hydrophobic TFC Membranes. ... 108
6.4 Conclusion. ... 110
Chapter 7. High Flux TFC Membranes with intrinsic microporosity by
interfacial polymerization for Organic Solvent
7.1 Introduction. ... 113
7.2 Experimental. ... 115
7.2.1 Materials. ... 115
7.2.3 Preparation of PEEK UF support membranes. ... 116
7.2.4 Preparation of network PIMs-like thin film composite membranes by IP. ... 116
7.2.5 Membrane performance. ... 118
7.3 Results and discussion. ... 119
7.3.1 TFC-PIMs-PI membrane performance. ... 119
7.3.2 TFC-PIMs-PEEK membrane performance. ... 123
7.4 Conclusion. ... 125
Chapter 8. High flux TFC OSN membranes for the purification of Active
Pharmaceutical Ingredients. ...127 8.1 Introduction. ... 127 8.2 Experimental. ... 128 8.2.1 Materials. ... 128 8.2.2 TFC membrane preparation. ... 128 8.3.3 Membrane performance. ... 128
8.3 Results and discussion. ... 129
8.3.1 Membrane Flux and Rejection. ... 129
8.3.2 Membrane Stability. ... 131
8.3.3 Separation of API/impurity and process comparison. ... 132
8.4 Conclusion. ... 134
Chapter 9. Final conclusions and future directions. ...135
9.1 Final conclusions. ... 135
9.2 Future directions. ... 136
Research motivation and thesis structure
A challenge for nanofiltration (NF) and reverse osmosis (RO) is to broaden their application range from aqueous to organic feeds. Industries from oil refining to pharmaceuticals could reap major benefits from reduced energy consumption and simplification of solvent based processes, just as the desalination industry has benefitted from the introduction of reverse osmosis membranes. Meeting this challenge requires solvent stable membranes that preserve their separation characteristics in a wide range of solvents, and which offer defect-free morphology and controlled molecular weight cut-offs (MWCOs). Organic Solvent Nanofiltration (OSN) is an emerging technology for molecular separation and purification processes carried out in organic solvents , based on selective solvent stable membranes.
Many of the OSN membranes developed to date are integrally skinned asymmetric membranes prepared by the Loeb-Sourirajan method [1, 2]. These integrally skinned asymmetric membranes suffer from limitations in terms of flux for some organic solvents, and tight membranes (MWCO=150-300 Daltons) have poor fluxes in polar and non-polar solvents. This limitation might be overcome by carefully controlling the formation of the separation layer. Another possibility is to adopt a more sophisticated strategy: develop Thin Film Composite (TFC) membranes via interfacial polymerization (IP) for OSN applications. TFC membranes (first developed by Cadotte ) consist of an ultra-thin “separating barrier layer” prepared via IP on top of a chemically different porous support, which gives more freedom to design an effective membrane for a specific application.
Conventional TFC membranes used for aqueous applications cannot be used in strongly swelling solvents because the membrane supports tend to swell or dissolve, affecting the membrane separation performance. Thus, the solvent stability of TFC membranes must be improved. The aim of this thesis is to develop TFC OSN membranes via IP for polar and non-polar solvents. The hypothesis of this work is that TFC OSN membranes have the potential to achieve higher fluxes than integrally skinned asymmetric OSN membranes, without sacrificing selectivity. However, to
date there are no reported TFC OSN membranes prepared via IP which are stable in strongly swelling solvents, such as polar aprotic solvents, including DMF and THF.
Conventional purification technologies in the manufacture of Active Pharmaceutical Ingredients (APIs) include crystallisation, distillation, liquid-liquid extraction, chromatography, and adsorption onto activated carbon or silica. However, they have limitations in cost, scale up and selectivity. During the production of APIs harsh organic solvents of different polarities are used. Thus, stable membranes with controlled polarity are required. In order to make this process viable and versatile, new polymeric and ceramic OSN membranes with high selectivity, improved permeability and tuneable polarity need to be developed.
To date, there is no research evidence in the use of TFC OSN membranes to purify active pharmaceutical ingredients. However, such an OSN process, in principle, could be employed. This work will focus on developing a new generation of OSN membranes: High flux TFC OSN membranes via interfacial polymerization. As a result, a cheaper, more selective and more efficient process for the removal of impurities during the manufacture of APIs could be developed.
It was decided to try different chemistries to make defect-free films by interfacial polymerization as the TFC top layer. These films should be resistant in organic solvents and have good permeance in polar or non-polar solvents. Once these chemistries were selected, the properties of the supports on the overall TFC membrane performance were studied and a real API purification was carried out as a proof of concept.
It is possible to prepare different polymer chemistries by interfacial polymerization. In Chapter 4, polyamide was the selected chemistry to prepare the top layer of hydrophilic OSN TFC membranes for polar solvents as the formed polyamide and the monomers used present several advantages compared to other polymer systems: (a) polyamide network is stable in many organic solvents; (b) the interfacial polymerization reaction to form polyamide is fast, forming a thin film instantly avoiding the formation of defects; (c) the chosen amines (MPD, PIP and HDA) used to make polyamide are soluble in water and can diffuse to the organic phase (hexane) easily; (d) the selected amines and acyl chloride are commercially available. Several attempts to polyethers top layer by interfacial polymerization failed because the reaction was very slow; the film formed after several days. In Chapter 4, novel high flux hydrophilic TFC OSN membranes were developed via interfacial polymerization on crosslinked polyimide support. Different parameters during the TFC membrane formation where studied and controlled, to achieve higher permeability without compromising selectivity. Their MWCOs were controlled by using different amines during the IP reaction. To prove the potential of these TFC membranes for the purification of APIs in polar
solvents, in collaboration with Elin Rundquist (GSK), a purification study is described in Chapter 8. To ensure TFC membranes can be used in non-polar solvents, a detailed analysis on surface modification and incorporation of hydrophobic monomers during the IP reaction was undertaken in Chapter 5 to find an optimum method to render the TFC membranes hydrophobic. In Chapter 6, the effect of the support membrane on the overall TFC membrane performance in polar and non-polar solvents was studied. Two different solvent stable supports were developed for the formation of both hydrophilic and hydrophobic TFC membranes. A detailed study on the morphology, porosity, surface chemistry and polarity of each support was undertaken to understand the influence of these parameters on TFC membrane formation and performance. Finally, in Chapter 7 to further enhance permeability a PIM-like network polyester was formed as the top layer of TFC OSN membranes. A contorted monomer was used during the IP reaction to provide concavity and higher porosity to the top layer. Polyester being more hydrophobic than polyamide would perform well in both polar and non-polar solvents. It is also stable in many organic solvents and the formation of the film is instantaneous, resulting in a defect-free top layer. The effects of curing on TFC membrane performance were studied to find an optimum MWCO without compromising permeability. The performance of these ultra high flux PIM-like membranes was compared with commercial integrally skinned asymmetric membranes and with the TFC OSN membranes prepared in Chapters 5 and 6.
This review seeks to provide insight into state-of-the-art research in TFC membranes for both aqueous and organic applications, as well as into how different parameters in the membrane formation and post-formation processes affect overall membrane performance.
Currently, in RO and NF applications, membranes with very thin top layers are used. Membranes displaying this combination of a separating top layer on a more porous support structure are called asymmetric membranes. These membranes will be explained in further detail in section 2.2.
Phase inversion, developed by Loeb and Sourirajan  in the early sixties, is one of the most adaptable, economical and reproducible techniques for the formation of asymmetric polymeric membranes. These membranes possess a skin-layer on top of a more porous sublayer with the same chemical composition as shown in Figure 1(a), and are often called integrally skinned asymmetric (ISA) membranes. The key for high performance is the thin skin-layer, which makes higher selectivity possible. Another important class of membranes, effective for RO and NF, are TFC membranes developed by Cadotte . They consist of a thin “separating barrier layer” on top of a chemically different porous support as shown in Figure 1(b). The separating layer of TFC membranes is normally prepared via dip-coating or by interfacial polymerization on a support-layer, which is formed by phase inversion. Because of their layered structure, TFC membranes are very flexible and the chemistry and performance of both barrier-layer and porous substrate can be independently optimized to maximize overall membrane performance [3, 8, 7].
In general, attention has been on the development of TFC membranes for aqueous applications, in particular sea water desalination. However, these membranes can also be used for filtrations in certain organic solvents and, with some optimization, in a wider range of solvents.
Figure 1. Schematic representation of polymeric membranes; (a) integrally skinned asymmetric membrane; (b) thin film composite membrane.
2.1.1 Membrane development for reverse osmosis
Figure 2 shows the performance of important RO membranes produced for the desalination market. The dotted line at 99.3 in the plot, divides the figure in two sections. This value is the minimum sodium chloride rejection that can produce potable water from seawater in just one pass . Only Cellulose triacetate, PEC-1000 and some types of cross-linked fully aromatic polyamides can fulfil this requirement. However, cellulose triacetate has lower fluxes and deteriorates in water. Thus, the only types of RO membranes that can efficiently produce potable water in a single pass from sea water are cross-linked polyether and cross-linked fully aromatic polyamide membranes. This is one of the reasons why most
development has been focussed on polyamide TFC membranes.
The first asymmetric RO membranes, prepared by Loeb and Sourirajan at the beginning of 1960s, showed a water flux 100 times higher than any symmetric membranes known . This development enabled the successful commercialisation of reverse osmosis membranes. In 1970, cellulose acetate membranes
were the first type to be commercially available . One of the main disadvantages of cellulose acetate membranes is their deterioration due to hydrolysis, which is strongly dependent on the pH of the feed. Therefore, careful pH control and adjustment is needed. Another disadvantage of these membranes is that they tend to compact under high pressure, decreasing their flux as well as their overall performance .
Figure 2. RO membranes performance (adapted from ). (b)
Cellulose acetate membranes are still commercially available. However, they are being increasingly replaced by TFC membranes (e.g. PEC 1000, and cross-linked polyamide membranes), which have a high physical stability, since the skin layer is chemically bonded to the support.
Thin film composite membranes can be prepared by different methods, which will be explained later in this chapter. The most developed one is interfacial polymerization, a technique invented by Cadotte [10, 11, 12] which allows the production of polymer layers down to 50 nm thick. Since this discovery, this method has become the new industry standard in reverse osmosis .
Interfacial TFC membranes have significantly higher salt rejections and fluxes than cellulose acetate membranes, with less than half the salt passage and two times the water flux . TFC membranes are physically and chemically more stable, possess strong bacterial degradation resistance, do not hydrolyse, are less influenced by membrane compaction and are also stable in a wider range of feed pH (3-11). Nevertheless, composite membranes are less hydrophilic and as a consequence, they are more prone to fouling than cellulose acetate membranes in RO applications, and deteriorate in the presence of very small amounts of free chlorine in the feed solution .
2.1.2 Influence of external parameters on membrane performance
In order to be efficient, membranes should present high flux and high solute rejection. Very thin membrane separation layers are required to achieve high permeability because flux is inversely proportional to the membrane thickness.
Solvent flux is proportional to the applied pressure gradient. Selectivity can be measured in a number of ways, but conventionally, it is measured as the solute rejection coefficient R.
Solvent flux (J) is determined by measuring permeate volume (V) per unit area (A) per unit time (t) according to equation 1. The rejection coefficient (Ri) is a measure of the ability of the membrane
to separate a solute i from the feed solution and is calculated from equation 2, where CP,i and CF,i
correspond to marker concentrations in the permeate and the feed respectively.
In membrane separation some general rules apply as follows :
1. when the operating pressure is increased the solvent flux first increases almost linearly, levels off as the pressure is raised further, and finally may even decrease at elevated pressure;
2. flux decreases as the solute concentration is increased;
3. at higher concentrations rejection strongly decreases and overall efficiency goes down.
2.2 Polymeric membranes
2.2.1 Integrally skinned asymmetric membranes
ISA membranes present a layered structure in which the porosity, pore size, and membrane composition change from the top to the bottom surface of the membrane. They have a thin selective layer supported on a much thicker, highly permeable microporous substrate of the same material. Because the selective membrane is very thin, membrane fluxes are high. The microporous substrate is essential as it offers the strength required for handling the membrane . Depending on the preparation conditions, these membranes can be used for ultrafiltration or nanofiltration applications.
ISA membranes can be prepared in the ultrafiltration range and used as support membranes for TFC membrane formation. They are made by the wet phase inversion technique , which involves the precipitation of a casting solution by immersion in a nonsolvent (water) bath. Water adsorption and loss of solvent cause the film to rapidly precipitate from the top surface down. A casting solution consisting of only one phase is precipitated into two phases: a solid, polymer-rich phase that forms the matrix of the membrane and a liquid, polymer-poor phase that forms the membrane pores .
In solution casting, a uniform film of an appropriate polymer is spread across a non-woven fabric (see figure 3). The casting knife comprises a steel blade, resting on two runners, arranged to form a precise gap between the blade and the plate onto which the film is cast. After casting, the film is precipitated by immersion in a water bath. Water precipitates the top surface of the cast film rapidly, forming the dense, selective layer. This layer slows the entry of water into the underlying polymer solution, which precipitates much more slowly and forms a more porous substrate. The thickness of the dense skin varies from 0.1 to 1.0 µm and it depends on the casting solution, the polymer, and other parameters. The thermodynamic properties of the system and the kinetics involved in the exchange of solvent and non-solvent have an impact on the membrane morphology, affecting its permeability and solute rejection .
Figure 3. Membrane casting.
The dope solution should be sufficiently viscous; usually polymer concentrations are in the range of 15 - 25 (w/w) % . The best solvents for dope solutions are aprotic solvents such as dimethylformamide, which can dissolve a large variety of polymers. Dope solutions based on these solvents precipitate rapidly when immersed in water to give porous ISA membranes.
2.2.2 Thin Film Composite membranes
Because of their layered structure, TFC membranes are very flexible and the chemistry and performance of both barrier-layer and porous support can be independently optimized to maximize the overall membrane performance [3,7,8].
The main methods for the formation of the top-layer of TFC membranes are : (a) casting an ultrathin film separately, then laminating it onto a support; (b) interfacial polymerization at the surface of a support; (c) dip-coating/solvent casting a solution of a polymer onto a support; (d) dip-coating a solution of a reactive monomer or pre-polymer onto a support, followed by a post-curing with heat or irradiation; (e) depositing a barrier film directly from a gaseous phase monomer plasma.
TFC membranes for organic solvent applications have been prepared using dip-coating. Currently, mostly all TFC RO membranes are prepared by interfacial polymerization (IP) and a lot of work has been done to understand the effect of different preparation parameters on the membrane's performance.
2.2.3 Post-treatment of polymeric membranes
Post-treatment procedures can be applied to both types of polymeric membranes: ISA and TFC membranes. In order to increase the long term stability of ISA membranes and to enhance their separation performance, various conditioning or post-treatment methods can be used, such as crosslinking, wet or dry annealing, drying by solvent exchange, and treatment with conditioning agents . Post-treatment is also crucial for polymeric ultrafiltration (UF) supports used to prepare TFC membranes . It is also possible to further enhance the performance of TFC membranes
by applying an appropriate post-treatment method . Several techniques to enhance membrane performance have been reported in the literature, including curing, grafting, plasma, UV and chemical treatment . More details on the curing and chemical post-treatment methods for TFC membranes can be found elsewhere [18 -24].
2.2.4 Advantages of TFC over ISA nanofiltration membranes
In aqueous applications, interfacial composite membranes have significantly higher salt rejections and fluxes than ISA cellulose acetate membranes. Typical TFC membranes, tested with 3.5 % sodium chloride solutions, have a salt rejection of 99.5 % and a water flux of 51.0 Lm-2h-1 at 55 bar (0.9 Lm-2h-1bar-1); this is less than half the salt passage and two times the water flux of cellulose acetate membranes .
In the last decades, a significant increase in membrane performance with respect to permeability and salt rejection can be observed. In 1981, Cadotte  reported flux values of 43 (Lm-2h-1) for composite membranes at standard test conditions (3.2 % NaCl, 55 bar, 25° C, 8 % recovery), while membranes today reach flux values of as high as (201 Lm-2h-1) . These values are accomplished with brackish water of low salinity, and for seawater membranes classical flux values are significantly lower. From 1996 to 2007, typical seawater membranes increased their rejection from 99.6 % to 99.8 %, whereas flux increased from 43 (Lm-2h-1) to 69 (Lm-2h-1) . An advantage of TFC membranes is that the thin barrier layer can be optimized for the desired flux and solute rejection, while the porous support can be optimized for maximum strength and compression resistance, and a minimum resistance to permeate flow. Moreover, the thin barrier layer can be formed from a large variety of chemical compositions, including both linear and crosslinked polymers, whereas the asymmetric membrane formation process is quite limited to linear, soluble polymers. Only a few of such linear polymers have the right combination of flux and solute rejection characteristics to generate commercially attractive membranes .
A disadvantage of TFC membranes is that their manufacturing is more expensive compared to ISA membranes. However, the extra cost of manufacturing TFC membranes is more than counterbalanced by the improved performance characteristics of the resulting membrane products . Similarly to water desalination, TFC OSN membranes have the potential to achieve higher fluxes than ISA OSN membranes, without sacrificing selectivity.
Producing an ultrathin layer in situ on a microporous substrate also allows the use of a variety of cross-linked polymeric compositions, which can present higher hydrophobicity or hydrophilicity for OSN applications as well as higher chemical resistance compared to linear polymers.
2.3 TFC membranes prepared by interfacial polymerization
These membranes are made by interfacially polymerizing a thin layer of polymer at the surface of a porous support membrane. Some general aspects of support membranes for solvent resistant TFC membranes will be discussed later (see section 2.5.3).
In IP, an aqueous solution of a reactive monomer, such as amine (hydrophilic monomer), is first deposited in the pores of a porous support membrane, usually a polysulfone ultrafiltration membrane. Then, the polysulfone support loaded with amine is immersed in a water-immiscible solvent solution containing a reactant, such as triacid chloride in hexane (hydrophobic monomer) (see Figure 4). The two monomers react at the interface of the two immiscible solutions, until a thin membrane film presents a diffusion barrier and the reaction is completed to form a highly cross-linked thin membrane layer that remains attached to the substrate. The thin layer can be from several tens of nm to several µm thick [3, 8, 25].
The dense, cross-linked polymer layer can only form at the interface, and as it is thin on the order of 0.1 µm or less, the membrane permeability is high. Because the polymer is highly cross-linked, its selectivity is also high. Even though the crosslinked interfacial polymer layer determines membrane selectivity, the nature of the porous UF support membrane affects membrane flux considerably. The film must be finely porous to stand the high pressures applied but should also have a high surface porosity so it is not obstructing solvent flow .
A large number of IP TFC membranes have been successfully developed consisting mainly of a polyamide (PA) top-layer, but poly(amide imide) (PAI), poly(ether amide) (PEA), polyurea and poly(urea amide) (PUA) TFC membranes have been developed as well .
The development of the FT-30 membrane by Cadotte was very important as it made single-pass seawater desalination with TFC membranes possible, and is the best commercial TFC membrane available for RO . It was produced by the reaction of m-phenylenediamine with trimesoyl chloride, shown in Figure 5. This membrane consists of an all-aromatic, highly crosslinked structure giving exceptionally high water flux and consistent salt rejections of 99.5 % from seawater .
Figure 5. Chemical structure of polyamide FT-30 membrane
In sections 2.3.2 to 2.3.4, the effect of different parameters during the IP reaction and membrane post-treatment on overall membrane performance will be explained in detail.
2.3.1 Theoretical model of interfacial polymerization
Interfacial polymerization takes place at an interface of two immiscible, low molecular weight fluids, each containing one of the reactants. The dissolved monomers diffuse to the interface, where they undergo the copolymerization reaction. The resulting copolymer is usually incompatible with either of the liquid phases and as a result, a polymer film grows at the interface.
The theoretical description [27,28] of the creation of a thin polymeric layer through interfacial polymerization specifically takes into account the effects of polydispersity on the formation of the polymer film at the liquid-liquid interface. Consequently, models [27,28] can predict both the kinetics of film formation and the molecular weight distribution of the polymer structure of the growing film. Predictions of the film thickness as a function of reaction time have been successfully related to experimental data.
To start the reaction the diamine partitions into the organic phase. It initially meets a high concentration of diacid chloride and is acylated at both ends. The following diamine molecules react with both the diacid chloride and the oligomers with acid functionalities at each end. The growing oligomer chains remain in the solution without precipitation as long as their concentration is less than their respective solubility limit in the organic phase. Phase separation of the oligomeric species starts when the concentration of the growing chains reaches the binodal of the oligomer-solvent phase diagram. Since the chains grow due to a fast reaction, it is assumed that phase separation starts when the concentration of the growing chains becomes equal to the spinodal concentration . Thus, there is some amount of super-saturation allowed before precipitation begins. After the spinodal is crossed, it is assumed that the precipitation of the chains occurs instantly.
The film that initially precipitates has the highest molecular weight. This high molecular weight stays constant for an extended period of time. However, the average molecular weight decreases as more oligomers of lower molecular weight exceed their solubility limit and start to precipitate, increasing the polydispersity of the polymer film. Hence, there is an optimum reaction time to get an adequately thick polymer film with a nearly constant high molecular weight .
2.3.2 Monomers used during IP to prepare TFC membranes
The thin layer formed via interfacial polymerization mostly consists of a polyamide crosslinked polymer, which is stable in a wide range of solvents including toluene, acetone, dimethylformamide (DMF), hexane and alcohols. Thus, the work reported on aqueous applications for membranes prepared via IP can be carried out in certain organic solvents. The trade-off between permeability and solute rejection in TFC membranes can be partially overcome by carefully choosing the monomers and the polymerization conditions [3, 29, 30].
Membranes prepared from aromatic diamines show better rejections, but lower fluxes compared to those prepared using aliphatic diamines. Thus, the former are typically used for RO-membranes, while piperazine or amine-substituted piperidines are preferred for NF applications . One of the main factors affecting rejection is the position of the acyl chloride and the amine groups on the aromatic rings. This has been shown for the reaction of o-, m- and p-phenylenediamine (OPD, MPD, PPD) with isophthaloyl or terephthaloyl chloride (IPC or TPC) [29, 30]. In the polyamide FT-30 membrane the triple functionality of the acyl compound results in a highly crosslinked, mechanically stable and selective network. Hydrolysis of the unreacted acyl groups can also
occur, leading to TFC membranes with fixed charges. This hydrophilization improves water fluxes, and at the same time decreases the density and rejection of the top-layer [29, 30].
In order to prepare loose RO or NF membranes, MPD is often blended with piperazine (PIP). This aliphatic diamine provides higher free volumes and larger pore sizes to the thin active layer .
The support is often relatively hydrophobic. However, the wettability of the support can be enhanced by adding wetting agents (e.g. polyethylene glycols (PEGs)) to the aqueous diamine solution . Furthermore, the overall membrane performance can be enhanced by adding
swelling agents (e.g. DMF), improving the interaction between the top-layer being formed and the swollen support .
Effect of amine structure
Previous work  studied the permeation performance of TFC membranes obtained from different diamines using TMC as the acyl chloride. All the thin films obtained showed a crosslinked structure. The thin films prepared with aliphatic diamines including 1,6-hexamethylenediamine (HDA), 1,9-nonamethylenediamine (NMDA) and dimethylenediamine (DMDA), had an aliphatic-aromatic network structure. However, the thin-films prepared with aromatic diamines including PPD and MPD had fully aromatic network structures. Network-structure polyamides showed a relatively high salt rejection compared to linear Network-structure polyamides. In the case of the membranes having aliphatic-aromatic network structures, the water flux and the salt rejection decreased with increasing length of the aliphatic methylene chain. On the other hand, thin films with fully aromatic network structures showed high salt rejection and relatively high water flux compared to membranes having aliphatic-aromatic network structures.
Furthermore, the polar component of surface tension was evaluated as a possible measure of the hydrophilicity of the thin active film . The polar force for the thin-films made from aliphatic diamines decreases as the methylene chain of the aliphatic amines increases in length.
Similar to amines, a broad range of aromatic acyl chlorides have been used to prepare polyamide (PA) based TFC membranes. The number and position of the acyl halide groups on the aromatic ring is a major factor affecting the salt rejection, as they determine the chain structure and the crosslinking degree of the PA network formed . The hydrolysis of acyl chloride groups to carboxylic acid groups has an important effect on the hydrophilicity, surface charge and degree of crosslinking of the membrane . In addition to acyl chloride monomers, polymers with acyl chloride pendant groups can be used. Mixtures of isophthaloyl chloride (IPC) with
poly(isobutylmethacrylate-co-aryloyl chloride) in combination with a tetrafunctional aromatic amine showed good film forming properties . The contact between the phases containing the reactive monomers was improved by replacing the organic phase with benzene or 1,2-dichloroethane, as these are better solvents for the formed PA polymer. By replacing the organic phase, rejections were significantly improved .
Effect of acyl chloride structure
Different properties of linear as well as network structures prepared using di/tri-functional aromatic and aliphatic acyl chloride monomers have been studied using MPD as the diamine. The di-functional acyl chlorides including sebacoyl chloride (SC), isophthaloyl chloride (IPC), and terephthaloyl chloride (TPC) result in a linear structure, whereas the tri-functional acyl chloride, TMC results in a network structure. SC results in an aromatic (amine)-aliphatic (acyl chloride) structure, but the polymers prepared using aromatic acyl chlorides including IPC, TPC, and TMC have a fully aromatic structure. The thin active films that had linear structures (SC, IPC, and TPC) had low salt rejection, whereas network structures (TMC) gave higher salt rejection. Thin active films with the aromatic-aliphatic linear structure (SC) showed high water fluxes, while fully aromatic linear structures (IPC and TPC) resulted in lower water fluxes .
The components affecting the polar force are an amide bond, an amine and carboxylic acid end-group, and a free carboxylic acid group in the network structure. The free carboxylic acid groups result in unreacted acyl chloride groups, which can easily be converted to the corresponding carboxylic acids through hydration. The polar forces of the thin polyamide films with fully aromatic linear structure are lower compared to the polyamide having aromatic-aliphatic linear structure .
Effects of polymerization parameters
Monomer concentration has a great influence on the performance of TFC membranes. Lu et al.  suggested that the key of the IP method was to select the right partition coefficient of the reactants in the two-phase solution and to set the appropriate diffusion speed of the reactants to achieve the ideal degree of densification of the membrane surface. Moreover, the concentration of the diamine is an important factor, which can affect the performance of the resulting membrane, since it may control the uniformity and thickness of the ultimate polyamide top-layer. Since the IP process is diffusion controlled in the organic phase , the effect of organic phase reactant is likely to have a great impact on membrane performance.
Higher monomer concentrations [22, 31, 37], higher reaction rates  and longer polymerization times [22, 31, 37] generally improve the efficiency of film formation. These result in thicker and
denser barrier-layers with increased rejections but decreased fluxes. As the concentration of the monomers increases, the thickness of the barrier-layer also increases. The polymerization reaction takes place at the interface between both phases, but the nascent film then gradually grows away from the aqueous phase as the amines diffuse through the interface and the film being formed. As the reaction continues, the film thickness will prevent further amine-diffusion and stop film growth .
In previous work , the effect of TMC on the membrane properties was studied based on the piperazine/3,5-diaminobenzoic acid (PIP/BA) system. In the case of nanofiltration membranes, it is speculated that the TMC content has a high impact on the rate and degree of reaction, which eventually affects the final performance of the membrane. The relationship between PIP/BA and TMC systems were studied. As the concentration of TMC content is increased, the pore size is reduced. TMC content plays an important role in determining the rate of reaction, while the reaction time will determine the extent of reaction. For short reaction time (5s), the extent of crosslinking is low, and the pore size produced (calculated using the Donnan Steric Pore Flow Model) is larger (0.74nm) . However, when the concentration of TMC is increased, the rate of reaction is increased tremendously. In the case of PIP/BA mixtures, its reduced reactivity produces a more porous structure. It was also found that at higher BA ratio to PIP, the pore size produced is bigger. The increases in rejection at 0.10 % TMC and 0.15 % TMC are due to the decreasing pore size as a result of crosslinking. However, it was observed that the rejection performance dropped at high-TMC content (0.20 %), because pore loosening starts to occur where the reaction rate is so high that excessive 3,5-diaminobenzoic acid is introduced . Skin layers with higher BA content produce membranes with loose structures.
Effects of soaking time on TFC membrane performance
It is known that with the soaking time being prolonged, the top layer in the TFC membranes thickens, the rejection of the TFC membrane increases, and flux decreases . The polycondensation reaction between amine and acid chloride is exothermic, and so the reaction rate increases with increasing temperature, increasing the extent of crosslinking .
Solubility of the monomers
Prior to the preparation of the TFC membranes, the solubility of the monomers should be determined in order to select appropriate solvents for the acyl chloride solution that do not solubilise the UF support membranes .
When the two monomer solutions are brought into contact, both monomers partition across the liquid-liquid interface and react to form a polymer. However, polymerization occurs predominantly